Simple Route to Obtain Nanostructured CeO2 Microspheres and CO Gas Sensing Performance
© The Author(s). 2017
Received: 16 December 2016
Accepted: 26 February 2017
Published: 6 March 2017
In this work, nanostructured CeO2 microspheres with high surface area and mesoporosity were prepared by the coprecipitation method, in absence of a template. The reaction between cerium nitrate and concentrated formic acid produced cerium formate, at room temperature. Further, calcination at 300 °C yielded single-phase CeO2 microspheres, with a diameter in the range 0.5–2.6 μm, the surface of these microspheres is completely nanostructured (diameter about 30–90 nm). CeO2 microspheres were used to fabricate a sensor device, and it was tested for intermediate CO gas concentrations (200–800 ppm). The detection of 200 ppm carbon monoxide was observed at 275 °C, with a response time of 9 s, using an applied frequency of 100 kHz. The detection of changes on the CO gas concentration was studied at different temperatures and applied frequencies. The results revealed a reproducible and stable gas sensing response.
KeywordsCeO2 Coprecipitation Microspheres Gas sensor
Cerium oxide (CeO2) is one of the most reactive rare earth oxides, with unique physical and chemical properties, such as oxygen storage capacity, oxygen deficiency, and electronic conductivity [1–4]. These characteristics have allowed CeO2 to be widely used in catalysis, energy storage, biosensors, among others [5–10]. In recent years, CeO2 has also been investigated as gas sensor; Izu et al. used the mist pyrolysis method to prepare CeO2 at 700 °C. Here, a powder with an average particle size of 200 nm and a random network structure was obtained . In this study for a comparative purpose, CeO2 with average particle sizes of 200 and 2000 nm was used to fabricate a resistive oxygen gas sensor. They concluded that the response time (8 s) for the sensor with smaller particle size (200 nm) was approximately one-tenth of the time taken by the sensor with a larger particle size (2000 nm) at 712 °C. Moreover, when the sensor kinetics is controlled by the diffusion of oxygen vacancies, the response time varies with the particle size. These conclusions were supported in a previous work reported by Beie et al. . Xie et al. who obtained CeO2 nanoparticles (10–15 nm) at 500 °C using a solvothermal method . They used these nanoparticles to prepare a humidity sensor device. In a humidity range of 11–98% (relative humidity, RH), the response and recovery times were 10 and 3 s, respectively. In addition, two sensing mechanisms were reported. At low RH, the process is given by conduction and polarization of the grains of CeO2, whereas at high RH, the conduction process is attributed to decomposition and polarization of the absorbed water.
In recent decades, there has been an ever-increasing demand for gas sensors. CO has attracted the attention for its monitoring due to the health risks caused by prolonged exposure to this gas. Some of the characteristics of CO are colorless, odorless, tasteless, and non-irritating but lethal. CO is a poisonous gas produced by the incomplete burning of carbon-based fuels. At concentrations below 200 ppm, this gas induces slight headache and dizziness. In a range between 200 and 400 ppm, the exposure to CO promotes a slight headache and loss of judgment. At 800 ppm, the health risk is greater (dizziness, nausea, and convulsions), being lethal at 12800 ppm with only 3 min of exposure .
Several semiconductor materials have been tested as CO gas sensor; SnO2 is one of the most tested materials for this purpose [15–18]. CeO2 has also been tested as a CO sensor though low (<100 ppm) or high (>1000 ppm) is usually reported. At low CO gas concentrations, Itoh et al. used zirconium-doped cerium oxide to prepare a sensor device . This device was tested in CO concentration in a range between 0.1 and 2 ppm though no details for response time were given. Durrani et al. used CeO2 commercial pellets to obtain thin films at 500 °C as sensor device . To study the CO gas sensing response, operation temperatures in the range 300–500 °C and gas concentrations between 500 and 50,000 ppm were tested. With these conditions, they found that the optimum operating temperature was around 390 °C and the response and recovery time were 45 and 25 s, respectively. Izu et al. studied CeO2 thick films using Pt/alumina as a catalyzer; different synthesis temperatures were tested in the range 800–1100 °C . The best result was obtained at 450 °C using 5000 ppm. The response time was 2 s with an average particle size of 58 nm.
The most important parameters involved in the detection of gas species are the operating temperature, sensitivity, selectivity, and long-term stability. These can be improved in a material by decreasing its particle size to the nanometer scale, as well as an increase in the porosity . According to what several authors have reported [23–25], the sensitivity of a material is reciprocal to the grain size as long as the depletion region extends over the grain. Thus, there is an importance to get a grain size twice smaller than the depletion layer thickness, and this occur when the grain size is in a nanometer scale (D < 2 L, L = depletion layer). As the grain size is smaller, a higher surface area is obtained. To maximize the specific surface area, the particles should be loosely packed; then a very small contact area between each other is obtained. This is obtained with spherical or semispherical morphology. However, to improve the gas sensing performance, an excellent connectivity between the grains is necessary. In this point, the synthesis temperature plays a key role. If the material is synthesized at high temperature, the grain size increases as well as the connectivity between them. However, the surface area decreases, and given that the gas sensing mechanism is surface area dependent, we will have an effect in this phenomenon. For porous materials, the gas is easy to be diffused into the bulk, which promotes the rapid response and recovery of the sensor. In addition, when a material is mesoporous (2 nm < pore radii < 50 nm), the gas transport occurs by molecular diffusion, whereas if the material is microporous (pore radii < 1 nm), the gas transport becomes a surface diffusion. So, it is also important to control the morphology.
With this purpose, CeO2 has been synthesized by numerous methods where different chemical agents were used. To mention some, Xu et al. synthesized broom-like porous CeO2 hierarchical architecture by hydrothermal method . For this synthesis, dihydrate trisodium citrate, urea, and cerium nitrate hexahydrate were used. The optimum reaction time and temperature were 39 h and 120 °C, respectively. Surface area values between 30 and 166 m2/g were reported. Large-scale CeO2 nanowires were prepared using the sol-gel method process at 600 °C by Wu et al. where porous anodic alumina template and cerium nitrate hexahydrate were used . Micro- and nano-sized spheres have been obtained with different precursor materials. For example, Liu et al. fabricated mono-dispersed CeO2 hallow nanospheres at 300 °C; with an average size in the range of 50–200 nm, surface area value of 61 m2/g and pore size of 50 nm were obtained . In this synthesis, tetrahydrate sulfate cerium and ammonium were employed. In addition, CeO2 microspheres were obtained at 600 °C by Feng et al.; cerium nitrate hexahydrate, potassium sulfate, and nitric acid were used for this purpose; surface area value of 15.6 m2/g was reported .
In a previous work, hierarchical 3D architectures of CeO2 were obtained at 400 °C by the microwave-assisted coprecipitation method. For this synthesis process, these were used ceric ammonium nitrate and formic acid as precursor materials. The morphology of the samples obtained from 170 to 600 °C was composed of hollow microspheres, with a size between 1.5 and 10 μm. These powders were used to fabricate CO gas sensor devices. As a general trend in gas sensing characterization, no steady state was observed and the response time was at least 20 s .
In the present work, to study the effect on microstructure and synthesis temperature, a similar synthesis method was employed to prepare CeO2, but cerium nitrate was used instead of ceric ammonium nitrate. The first aim in this work was to get CeO2 at lower temperature and with this an increase in the surface area, which will be seen in the sensor device performance. The sensing characterization was carried out at lower temperature than in the previous work. The effect of the cerium nitrate in the morphology was analyzed by FESEM. Moreover, the surface area and pore size were determined by the BET method. The gas sensing behavior was analyzed using an alternating current (AC), with different operational temperatures, frequencies, and gas concentrations. The second aim was to get stable electrical measurements; both aims were achieved.
All reagents used in this work were analytical grade and were used without further purification. The process to synthesize nanostructured CeO2 microspheres was the following: 0.76 g of cerium nitrate was dissolved into 10 ml of concentrated formic acid (>95%), under strong stirring. The resultant suspension was stirred for 24 h, at room temperature. Later, the solvent was evaporated intermittently using a domestic microwave oven, in steps of 40 s. The resulting material was dried overnight at 100 °C and later calcined to 200 and 300 °C for 5 h, in air.
The crystal structure was analyzed by X-ray powder diffraction (XRD), using an Empyrean (PANalytical) diffractometer, with Cu-Kα radiation (λ = 0.15418 nm), and diffuse reflectance FT-IR spectroscopy, using a Perkin-Elmer GX3 spectrometer, with samples dissolved in KBr. The surface area was determined by the Brunauer–Emmett–Teller (BET) method, and the pore size distribution was calculated by the Barrett–Joyner–Halenda (BJH) method, using desorption branch. Before measurements, the sample was vacuum degassed at 200 °C, for 12 h, using a TriStar II Plus apparatus.
The morphology of the samples was investigated by FESEM (Hitachi, SU8010) and HRTEM (FEI, Tecnai F30) with an accelerating voltage of 200 kV. No special treatment was applied for the FESEM analysis. The sample for TEM characterization was prepared by placing a drop of colloidal solution on carbon-coated copper grid and dried at room temperature.
Results and Discussion
FT-IR spectra of calcined samples are shown in Fig. 2b. Samples calcined at 100 and 200 °C show broad absorption bands of the asymmetric and symmetric stretching vibrations of OHO, placed at 3080–3700 cm−1. The IR absorption peaks at 2900 cm−1 are assigned to C–H stretching vibrations. The bands at 1650–1540 cm−1 and 1447–1340 cm−1 correspond to the asymmetric and symmetric stretching vibrations of the bound carboxylic groups (COO−). And the band at 780 cm−1 is related to the stretching vibrations of C–C groups. The spectra obtained from samples annealed at 200 and 300 °C show the characteristic band of Ce–O stretching vibrations, located at around 500 cm−1 . The spectrum of a sample calcined at 300 °C shows the presence of a small amount of organic matter.
From Fig. 5a, a response time (t res) of 9 s was determined, which corresponds to the elapsed time measured at the 90% of the variation of Δ|Z| in the tested gas. When CO is removed, Δ|Z| returned to its original value; recovery time (t rec) of 8 s was calculated analogous to t res. The recovery process is determined by two steps, oxygen re-adsorption from the ambient at the surface and re-oxidation of the oxide . Nanometric grain size and large grain boundary could enhance the rapid recovery time and the Δ|Z| value due to the adsorption of the oxygen on the surface. Figure 5b displays repeatability in the detection of CO, and this can be observed with the Δ|Z| value after several cycles, which indicates that |ΔZ| returns to its initial value and the CO adsorbed on the surface was reversible. A previous work  has shown that the response time was 47 s, at 250 °C, 100 Hz and 300 ppm of CO, and the results did not show a steady-state. For a comparative purpose, Izu et al.  prepared two samples of CeO2. The first named core–shell nanoparticles (with Au 4 wt%), and the second named precipitated nanoparticles. The average particle size was 30 nm for the sensor devices. The gas sensing performance was carried out at 450 °C. The results show that the sensor prepared using the core–shell nanoparticles exhibits a response time of 46 s whereas the response time of the sensor fabricated using the precipitated nanoparticles was 49 s as an average, when CO concentrations varies from 1% to 5000 ppm. The recovery time reported for the measurements was an average of 50 s. Durrani et al.  prepared thin film of tin oxide mixed with cerium oxide by physical vapor depositions; the films were annealed at 500 °C. When the film was exposed to 500 ppm of CO at 430 °C, the response time was 26 s and the recovery time was 30 s. The morphology reported was a well-separated conical nano columnar structure. In both works, the response and recovery time are much larger that obtained in this work where nanostructured CeO2 microspheres was used to prepared sensor device.
where C A is the concentration of the target gas, t is time, D k is Knudsen diffusion coefficient, x is distance (depth) from the top surface of the sensing layer, and k is rate constant. This means that the concentration of the oxygen in the film should decrease due to the surface reaction. D k can be expressed as a function of C A . Liu et al.  in a theoretical approach tested different gas concentrations and found an expression to response time (t res = 0.85 L 2/D). In these works, it was concluded that response time is dominated by sensor thickness (L) and diffusion coefficients (D); the last one depends on the gas concentration. The response times for 100 and 200 ppm are very closed and could follow this relation. However, as the difference is small, it could be attributed to experimental error. However, a different behavior was noticed. From Fig. 7a, an absence of the steady state was observed; the opposite occurs for Fig. 7b. For the two gas concentrations tested (100 and 200 ppm), when CO gas was pumped out, Δ|Z| recovered its initial value. This behavior was described by Wolkenstein in . A general description could be as follows: at the beginning of the process, there are not enough molecules of CO available to react with the surface oxygen adsorption sites. This changes after some seconds, when the CO molecules get adsorbed. Figure 7a shows in a graphical manner the described behavior. After that initial stage, the steady state is observed. In contrast, when CO concentration increases, more molecules react with oxygen vacancies. This is illustrated in Fig. 7b. This allows to observe the steady state when 200 ppm of CO was supplied and then a higher response is obtained. In both cases, the desorption is completely irreversible, which indicates that R returns to the original value. With this, neutral and charged particles are removed from the surface during desorption. Even more, this value was constant after several cycles which indicate a long-term stability.
where R 0 is the initial response, ω is the frequency, τ is the system time constant, and i is the imaginary unit. In addition, a decrease of noise was observed and this noise is known as flicker noise or 1/f noise. In addition, the effect of the temperature operation over response time was noticed. When measurements were carried out with the same conditions (100 kHz, 200 ppm; Figs. 7b and 8b), the response time increased slightly when the operating temperature decreased (266 to 225 °C, respectively). This effect was widely studied by Helwig et. al and is related with the changes in activation energy on the surface during adsorption and desorption process .
Nanostructured CeO2 microspheres with large surface area and mesoporosity were synthesized by the coprecipitation method at low calcination temperature. Compared to previous results obtained from CeO2 where hierarchical architectures were obtained, in our results, a narrower particle size distribution was obtained. Also, in this work, microspheres also displayed a uniform nanostructured surface morphology. The gas sensor device based on as-prepared CeO2 microspheres exhibited more stable electrical measurements, which were observed by the development of the steady state; slightly upper response time (t res) was obtained using a lower operating temperature and a good recovery performance. The improvement of the CO sensing response can be attributed to a larger porosity and less particle agglomeration of CeO2 microspheres.
This work was partially funded by Tecnológico de Monterrey, Campus Monterrey, through the Research Chair in Nanotechnology and Devices Design. C.R.M. is grateful to Coordinación General Académica of Universidad de Guadalajara, for partial financial support through the PRO-SNI 2015 program. The authors are thankful to Reina A. Mauricio-Sánchez (CINVESTAV-Querétaro) for assistance in the FT-IR measurements.
CRM and AHM-P performed the synthesis and gas sensing characterizations. ERL-M and AE-Z performed the structural characterizations, FESEM, and HRTEM analysis. ERL-M and CRM wrote the paper. All authors discussed the results and the implications of this manuscript. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Koelling DD, Boring AM, Wood JH (1983) The electronic structure of CeO2 and PrO2. Solid State Commun 47:227–232View ArticleGoogle Scholar
- Phokha S, Pinitsoontorn S, Chirawatkul P, Poo-arporn Y, Maensiri S (2012) Synthesis, characterization, and magnetic properties of monodisperse CeO2 nanospheres prepared by PVP-assisted hydrothermal method. Nanoscale Res Lett 7:425View ArticleGoogle Scholar
- Pfau A, Schierbaum KD (1994) The electronic structure of stoichiometric and reduced CeO2 surfaces: an XPS, UPS and HREELS study. Surf Sci 321:71–80View ArticleGoogle Scholar
- Johansson B (1978) Energy difference between trivalent and tetravalent metallic cerium and other f-elements: stability study of various lanthanide- and actinide-halides and -oxides. J Phys Che Solids 39:467–484View ArticleGoogle Scholar
- Miceli P, Bensaid S, Russo N, Fino D (2014) CeO2-based catalysts with engineered morphologies for soot oxidation to enhance soot-catalyst contact. Nanoscale Res Lett 9:254View ArticleGoogle Scholar
- Busquets MA, Sabaté R, Estelrich J (2014) Potential applications of magnetic particles to detect and treat Alzheimer’s disease. Nanoscale Res Lett 9:358View ArticleGoogle Scholar
- Abdelrahim MYM, Benjamin SR, Aguilera LMC, Rodríguez IN, Cisneros JLHH, Delgado JJ, Santander JMP (2013) Study of the electrocatalytic activity of cerium oxide and gold-studded cerium oxide nanoparticles using a sonogel-carbon material as supporting electrode: electroanalytical study in apple juice for babies. Sensors 13:4979–5007View ArticleGoogle Scholar
- Liu H, Liu H (2016) Preparing micro/nano core-shell sphere CeO2 via low temperatura route for improved lithium storage performance. Matt Lett 168:80–82View ArticleGoogle Scholar
- Umar A, Kumar R, Akhtar MS, Kumar G, Kim SH (2015) Growth and properties of well-crystalline cerium oxide (CeO2) nanoflakes for environmental and sensor applications. J Colloid Interf Sci 454:61–68View ArticleGoogle Scholar
- Temerk Y, Ibrahim H (2016) A new sensor based on In doped CeO2 nanoparticles modified glassy carbon paste electrode for sensitive determination of uric acid in biological fluids. Sensor Actuat B-Chem 224:868–877View ArticleGoogle Scholar
- Izu N, Shin W, Murayama M, Kanzaki S (2002) Resistive oxygen gas sensor based on CeO2 fine powder prepared using mist pyrolysis. Sensor Actuat B-Chem 87:95–98View ArticleGoogle Scholar
- Beie HJ, Gnörich A (1991) Oxygen gas sensor based on CeO2 thick and thin films. Sensor Actuat B-Chem 4:393–399View ArticleGoogle Scholar
- Xie W, Liu B, Xiao S, Li H, Wang Y, Cai D, Wang D, Wang L, Liu Y, Liu Q, Wang T (2015) High performance humidity sensors based on CeO2 nanoparticles. Sensor Actuat B-Chem 215:125–132View ArticleGoogle Scholar
- Fine GF, Cavanagh LM, Afonja A, Binions R (2010) Metal oxide semi-conductor gas sensor in environmental monitoring. Sensors 10:5469–5502View ArticleGoogle Scholar
- Srivastava RK, Lal P, Srivastava SK (1994) Sensing mechanism in tin oxide-based thick-film gas sensors. Sensor Actuat B-Chem 21:213–218View ArticleGoogle Scholar
- Rella R, Serra A, Siciliano P, Vasanelli L, De G, Licciulli A (1997) CO sensing properties of SnO2 thin films prepared by the sol-gel method process. Thin Solid Films 304:339–343View ArticleGoogle Scholar
- Bakin AS, Bestaev MV, Dimitrov DT, Moshnikov VA, Tairov YM (1997) SnO2 based gas sensitive sensor. Thin Solid Films 296:168–171View ArticleGoogle Scholar
- Endres HE, Göttler W, Hartinger R, Drost S, Hellmich W, Müller G, Braunmuch CB, Krenkov A, Perego C, Sberveglieri G (1996) A thin-film SnO2 sensor system for simultaneous detection of CO and NO2 with neural signal evaluations. Sensor Actuat B-Chem 36:353–357View ArticleGoogle Scholar
- Itoh T, Izu N, Akamatsu T, Shin W, Miki Y, Hirose Y (2015) Elimination of flammable gas effects in cerium oxide semiconductor-type resistive oxygen sensors for monitoring low oxygen concentrations. Sensors 15:9427–9437View ArticleGoogle Scholar
- Durrani SMA, Al-Kuhaili MF, Bakhtiari IA (2008) Carbon monoxide gas-sensing properties of electron-beam deposited cerium oxide thin films. Sensor Actuat B-Chem 134:934–939View ArticleGoogle Scholar
- Izu N, Nishizaki S, Itoh T, Nishibori M, Shin W, Matsubara I (2009) Gas response, response time and selectivity of a resistive CO sensor based on two connected CeO2 thick films with various particle sizes. Sensor Actuat B-Chem 136:364–370View ArticleGoogle Scholar
- Tiemann M (2007) Porous metal oxides as gas sensors. Chem Eur J 13:8376–8388View ArticleGoogle Scholar
- Xu C, Tamaki J, Miura N, Yamazoe N (1991) Grain size effects on gas sensitivity of porous SnO2-based elements. Sensor Actuat B-Chem 3:147–155View ArticleGoogle Scholar
- Barsan N, Koziej D, Weimar U (2007) Metal oxide-based gas sensor research: how to? Sensor Actuat B-Chem 121:18–35View ArticleGoogle Scholar
- Gao L, Cheng Z, Xiang Q, Zhang Y, Xu J (2015) Porous corundum-type In2O3nanosheets: synthesis and NO2 sensing properties. Sensor Actuat B-Chem 208:436–443View ArticleGoogle Scholar
- Xu B, Zhang Q, Yuan S, Zhang M, Ohno T (2015) Morphology control and characterization of broom-like porous CeO2. Chem Eng J 260:126–132View ArticleGoogle Scholar
- Wu GS, Xie T, Yuan XY, Cheng BC, Zhang LD (2004) An improved sol-gel template synthetic route to large scale CeO2 nanowires. Mater Res Bull 39:1023–1028View ArticleGoogle Scholar
- Liu S, Xie M, Guo X, Ji W (2013) Synthesis of CeO2 hallow nanospheres via redox reaction based self-templating approach. Mater Lett 105:192–195View ArticleGoogle Scholar
- Feng T, Wang X, Feng G (2013) Synthesis of novel CeO2 microspheres with enhanced solar light photocatalyic properties. Mater Lett 100:36–39View ArticleGoogle Scholar
- Michel CR, Preciado AHM (2014) CO sensor based on thick films of 3D hierarchical CeO2 architectures. Sensor Actuat B-Chem 197:177–184View ArticleGoogle Scholar
- Ferreira NS, Angélica RS, Marques VB, de Lima CCO, Silva MS (2016) Cassava-starch-assisted sol–gel synthesis of CeO2 nanoparticles. Matter Lett 165:139–142View ArticleGoogle Scholar
- Truffault L, Andrezza C, Santilli CV, Pulcinelli SH (2013) Synthesis of PTSH-modified CeO2 nanoparticles: effect of the modifier on structure, optical properties, and dispersibility. Colloid Surface A 426:63–69View ArticleGoogle Scholar
- Sing KSW, Everett DH, Haul RAW, Moscou L, Pierotti RA, Rouquerol J, Siemieniewska T (1985) Reporting physisorption data for gas/solid system with special reference to the determination of surface area and porosity. Pure Appl Chem 57:603–619View ArticleGoogle Scholar
- Xiong G, Luo L, Li C, Yang X (2009) Synthesis of mesoporous ZnO (m-Zno) and catalytic performance of the Pd/m-ZnO catalyst for methanol steam reforming. Energy Fuels 23:1342–1346Google Scholar
- Hung IM, Wang HP, Lai WH, Fung KZ, Hon MH (2004) Preparation of mesoporous cerium oxide templated by tri-block copolymer for solid oxide fuel cell. Electrom Acta 50:745–748View ArticleGoogle Scholar
- Clifford PK, Tuma DT. Characteristics of semiconductor gas sensors, I. Steady state gas response. Sensor Actuat. 1982/83;3:233-254.Google Scholar
- Brailsford AD, Yussouff M, Logothetis EM (1993) Theory of gas sensors. Sensor Actuat B-Chem 13:135–138View ArticleGoogle Scholar
- Gong H, Hu JQ, Wang JH, Ong CH, Zhu FR (2006) Nano-crystalline Cu-doped ZnO thin film gas sensor for CO. Sensor Actuat B-Chem 115:247–251View ArticleGoogle Scholar
- Chang JF, Ku HH, Leu IC, Hon MH (2002) The effects of thickness and operation temperature on ZnO:Al thin film CO gas sensor. Sensor Actuat B-Chem 84:258–264View ArticleGoogle Scholar
- Izu N, Matsubara I, Itoh T, Akamatsu T, Shin W (2013) CO response of sensor based on cerium oxide thick films prepared from clustered spherical nanoparticles. Sensors 13:3235–3261View ArticleGoogle Scholar
- Durrani SMA, Al-Kuhaili MF, Bakhtiari IA, Haider MB (2012) Investigation of the carbon monoxide gas sensing characteristics of tin oxide mixed cerium oxide thin films. Sensors 12:2598–2609View ArticleGoogle Scholar
- Gardner JW (1990) A non-linear diffusion-reaction model of electrical conduction in semiconductor gas sensors. Sensor Actuat B-Chem 1:166–170View ArticleGoogle Scholar
- Sakai G, Matsunaga N, Shimanoe K, Yamazoe N (2001) Theory of gas-diffusion controlled sensitivity for thin film semiconductor gas sensor. Sensor Actuat B-Chem 80:125–131View ArticleGoogle Scholar
- Liu Y, Huang P, Song H, Zhang G. Modeling of hydrogen atom diffusion and response behavior of hydrogen sensors in Pd-Y alloy nanofilm. Scientific Report 6:37043. http://www.nature.com/articles/srep37043
- Wolkenstein T. Electronic process on semiconductor surfaces during chemisorption. Consultants Bureau; 1991.Google Scholar
- Brophy JJ (1985) Basic electronics for scientists. McGraw-Hill, SingaporeGoogle Scholar
- Helwig A, Müller G, Sberveglieri G, Faglia G (2007) Gas response time of nano-scale SnO2 gas sensors as determined by the moving gas outlet technique. Sensor Actuat B-Chem 126:174–180View ArticleGoogle Scholar